TY - JOUR

T1 - Thermal expansion of deuterated hopeite, Zn-3(PO4)(2)center dot 4D(2)O

AU - Schofield, Paul F.

AU - Knight, Kevin S.

AU - Hodson, Mark E.

AU - Lanfranco, Anna M.

PY - 2007/7

Y1 - 2007/7

N2 - The lattice parameters extracted from Lebail analysis of neutron powder diffraction data collected between 2 and 300 K have been used to calculate the temperature evolution of the thermal expansion tensor for hopeite, Zn-3(PO4)(2)center dot 2H(2)O, Pnma,Z=4with a= 10.6065(4) angstrom, b = 18.2977(4) angstrom, c= 5.0257(2) A at 275 K. The a lattice parameter shows a negative thermal expansion, the b lattice parameter appears to saturate at 275 K while the c lattice parameter has a more typical positive thermal expansion. At 275 K, the magnitudes of the thermal expansion coefficients are alpha(a) = -1. 1(4) x 10(-5) K-1, alpha(b) = 2.4(9) x 10(-6) K-1 and alpha(c) = 3.6(2) x 10(-1) K-1. Under the conditions of these experiments, hopeite begins to dehydrate to the dihydrate between 300 and 325 K, and between 480 and 500 K the monohydrate is formed. The thermal expansion of the dihydrate has been calculated between 335 and 480 and at 480 K the magnitudes of the thermal expansion coefficients are alpha(a) = 1(2) x 10(-5) K-1, alpha(b) = 4(l) x 10(-6) K-1, alpha(c) = 4(2) x 10(-5) K-1, alpha(beta) = 1 (1) x 10(-1) K-1, and alpha(v) = 2(2) x 10(-1) K-1. The thermal expansion of hopeite is described in terms of its crystal structure and possible dehydration mechanisms for the alpha and beta modifications of hopeite are discussed.

AB - The lattice parameters extracted from Lebail analysis of neutron powder diffraction data collected between 2 and 300 K have been used to calculate the temperature evolution of the thermal expansion tensor for hopeite, Zn-3(PO4)(2)center dot 2H(2)O, Pnma,Z=4with a= 10.6065(4) angstrom, b = 18.2977(4) angstrom, c= 5.0257(2) A at 275 K. The a lattice parameter shows a negative thermal expansion, the b lattice parameter appears to saturate at 275 K while the c lattice parameter has a more typical positive thermal expansion. At 275 K, the magnitudes of the thermal expansion coefficients are alpha(a) = -1. 1(4) x 10(-5) K-1, alpha(b) = 2.4(9) x 10(-6) K-1 and alpha(c) = 3.6(2) x 10(-1) K-1. Under the conditions of these experiments, hopeite begins to dehydrate to the dihydrate between 300 and 325 K, and between 480 and 500 K the monohydrate is formed. The thermal expansion of the dihydrate has been calculated between 335 and 480 and at 480 K the magnitudes of the thermal expansion coefficients are alpha(a) = 1(2) x 10(-5) K-1, alpha(b) = 4(l) x 10(-6) K-1, alpha(c) = 4(2) x 10(-5) K-1, alpha(beta) = 1 (1) x 10(-1) K-1, and alpha(v) = 2(2) x 10(-1) K-1. The thermal expansion of hopeite is described in terms of its crystal structure and possible dehydration mechanisms for the alpha and beta modifications of hopeite are discussed.

U2 - 10.2138/am.2007.2099

DO - 10.2138/am.2007.2099

M3 - Article

SN - 0003-004X

VL - 92

SP - 1038

EP - 1047

JO - American mineralogist

JF - American mineralogist

IS - 7

ER -